**A Generalized van der Waals Model for Light Gas Adsorption **

**Prediction in IRMOFs **

Journal: *Physical Chemistry Chemical Physics*
Manuscript ID CP-ART-01-2019-000285.R1

Article Type: Paper Date Submitted by the

Author: 27-Feb-2019

Complete List of Authors: Kong, Lingli; University of Wyoming, Department of Chemical Engineering

Adidharma, Hertanto; University of Wyoming, Department of Chemical Engineering, Department of Petroleum Engineering

**Physical Chemistry Chemical Physics**

### ARTICLE

Received 00th January 20xx, Accepted 00th January 20xx DOI: 10.1039/x0xx00000x**www.rsc.org/**

**A Generalized van der Waals Model for Light Gas Adsorption **

**Prediction in IRMOFs **

### Lingli Kong

a_{ and Hertanto Adidharma*}

a
By making reasonable simplification to the structures of isoreticular metal-organic frameworks (IRMOFs) and defining important attractive regions of square-well potential, an adsorption model derived from the Generalized van der Waals partition function is proposed to describe the isotherms of light gas adsorption in IRMOFs. The simplification of the structures is based on the geometries of the accessible surfaces and the dimensions of the frameworks, and the locations of the attractive regions are defined by examining the distribution of the adsorbate molecules. Grand Canonical Monte Carlo (GCMC) simulation using the simplified structures with square-well potentials and the complete atomic structures with Lennard-Jones potentials and Coulombic potentials are performed and compared to verify the reliability of the simplification. The adsorption model proposed in this work can predict adsorption isotherms of IRMOFs accurately by calculating the adsorbed amounts in different attractive regions of the simplified frameworks. It is also demonstrated that the model with the five parameters fitted to the adsorption isotherm at one temperature can accurately predict the isotherms at other temperatures.

**1. Introduction**

Metal Organic Frameworks (MOFs) are highly porous materials with crystal structures. Due to their high storage capacity, selectivity ability, and thermal stability, MOFs are widely used for gas storage, gas separation, catalysis, and gas purification.1

Thus, obtaining the adsorption isotherms of different adsorbates, which contain important equilibrium information,2

is a crucial step to screen the best MOFs for different purposes. Experiments can always be performed to obtain isotherms, but they are usually costly and time consuming, and therefore experimental efforts should be minimized, and tools, such as molecular simulations and theoretical or engineering models, are commonly used to generate or predict isotherms.

Molecular simulation has been proven to be a powerful tool
for characterizing MOFs.3_{ Not only can it conduct the }

calculations and predictions based on the existing MOFs, but it
also offers scientists a tool to gain insight into the hypothetical
MOFs. GCMC simulation is commonly used for generating
adsorption isotherms of MOFs.4_{ However, if the complete }

atomic structures are used, this method highly relies on force
fields to obtain the parameters of the frameworks. The
standard organic force fields (e.g., the universal force field
(UFF)5_{ and Dreiding}6_{), which have been applied for conducting }

simulations, do not have universality for this capricious group of
materials.7_{ With high accuracy in representing the interaction }

potentials, the second order Møller-Plesset perturbation theory

(MP2) and density function theory (DFT) are commonly applied
to study the adsorption phenomena in MOFs, 8-10_{ including }

MOFs with open-sites.11, 12_{ However, }_{ab initio}_{ method is too }

expensive to be applied to large systems.13_{ Furthermore, it is a }

time-consuming process to conduct millions of cycles to
generate one point on the isotherms, not to mention the time
and the computation cost to screen thousands of millions of
possible MOFs, and strategies developed for large-scale
screening of MOFs are still based on large-scale simulations to
build database.14-18_{ Considering that the adsorbents used in }

simulations are rather ideal in structure conformations and purities, parameters obtained theoretically will also be less accurate in dealing with real MOFs, which have various structure defects.

Building simple but accurate models is one of the most
desirable tools for predicting adsorption isotherms. However,
the application of this idea to MOFs is still far from satisfactory.
It was suggested that heat of adsorption, surface area, and free
volume are different leading factors for the adsorption in
IRMOFs depending on the adsorption regimes at different
pressure ranges.19, 20_{ The existing adsorption models that have }

been applied to predict the adsorption phenomena in various
MOFs, such as Langmuir adsorption model, Tόth equation,
Dubinin-Astakhov (DA) equation, Dubinin-Radushkevich (DR)
model, Freundlich equation, and the modified versions of them,
are either based on multilayer mechanism, which is dependent
on surface area only, or pore-filling mechanism, which is
dependent on free volume only.21_{ Therefore, the good }

performance of these models cannot be guaranteed for different MOFs under different adsorption conditions. Multisite Langmuir model, which can take into account the effects of each selected adsorption site on the adsorption isotherms, is

*a. _{Department of Chemical Engineering, University of Wyoming, Laramie, Wyoming, }*

*82071-3295, USA. E-mail: adidharm@uwyo.edu*

† Electronic supplementary information (ESI) available: The simplified structure and the distribution of attractive regions.

considered to be more realistic because it considers the
conformations of the real MOFs, but the calculations of the
interaction energy terms still rely on *ab initio* method, which
means that the model is computationally expensive. 22,23

Researchers have also developed engineering models
specifically for the adsorption prediction in MOFs. The
Sanchez-Lacombe (SL) Equation of State (EOS) and Perturbed Hard
Sphere Chain (PHSC) EOS were applied to predict the isotherms
by calculating the adsorbate ‘solubility’ in MOFs.24-26_{ This type }

of model is simple in parameters, but it sacrifices the accuracy.
A semiclassical SAFT-VR-2D model was built for the adsorption
of a binary mixture of hydrogen and methane in MOFs.27_{ }

However, the model considers MOFs as structureless systems and the influence of the metal clusters and the organic ligands is ignored.

Since MOFs are materials of great variance in structure
topologies and building blocks, as the first step toward the
modeling of MOFs, we choose to model the adsorption in
IRMOFs, which have the same cubic topology with different
pore functionalities and sizes.28_{ Since the functional groups, }

such as -Br (IRMOF-2), -NH2 (IRMOF-3), -OC5H11 (IRMOF-5), etc.

can lead to chemisorption and dramatically influence the adsorbed amount of some certain gases, we do not discuss this type of IRMOFs. In this work, we propose an adsorption model that considers atoms in different parts of the structure as

different groups that can generate attractive regions of square well potential. The adsorbed amount can be obtained by predicting the density of the adsorbate in each attractive region independently. Square-well potential is applied to the adsorbate/adsorbate and adsorbate/adsorbent interactions, which is achieved by implementing structure simplifications.

Considering that there is not enough experimental data
available for the adsorption of different gases in different
IRMOFs, we use RASPA 2.029_{ to generate adsorption isotherms }

of IRMOFs as realistic references for testing the reliability of the simplifications and examining the performance of the proposed model. Developed at Northwestern University with collaboration from the University of Amsterdam, the University Pablo de Olavide, and the University of Delft, RASPA code is mainly utilized in the area of thermodynamic properties of liquids and gases, and adsorption/diffusion behavior of adsorbates in crystalline nanoporous materials. The results generated by RASPA are considered to be high in correctness and accuracy because of the implementation of advanced techniques and algorithms, e.g., configurational-bias Monte Carlo (CBMC) and continuous fractional component Monte Carlo (CFCMC). Verified by data generated from experiments and RASPA 2.0 software, we will show that the model can accurately predict isotherms at different temperatures by using parameters fitted to one isotherm. We will also prove that the

(a) IRMOF-1 structure and accessible surface.

Red spheres represent oxygen (O) atoms, turquoise spheres represent carbon (C) atoms, white spheres represent hydrogen (H) atoms, and brown spheres represent zinc (Zn) atoms.

(d) Cubic attractive region of the simplified corner. (e)Attractive region around the linker prism.

**Fig. 1** Simplified structure and attractive regions of IRMOF-1

(b) Simplified cuboid model of the

**Physical Chemistry Chemical Physics**

** ARTICLE**

model also works for the adsorption prediction of quadrupolar gases, such as CO2 and N2.

**2. Modeling**

**2.1 Simplified structure and attractive regions**

In this section, we describe how we simplify the IRMOF structures, which will lead to the development of our engineering model. IRMOFs are cubic networks constructed by Zn4O metal clusters and dicarboxylate linkers.30 Due to their

conformations, the shapes of void spaces in IRMOFs are irregular, and thus adsorption predictions based on models in cylindrical pores or slit pores are less reliable. We use RASPA 2.0 to generate data for the accessible surface of IRMOF-1 and visualize the results using the VTK software. Based on the shape of the accessible surface (Fig. 1(a)), we simplify the benzene ring and the ring formed by the dicarboxylate and the metal cluster to cuboids. The corner constructed by cuboids and the linker cuboid are shown in Fig. 1(b).

In the tiny space of the framework cell, both the metal atoms and the organic atoms of the frameworks generate attractive force. Thus, the force fields in the frameworks can be complicated, which makes it a tough task to build a simple engineering model for predicting the adsorption in IRMOFs, yet the distribution of the adsorbates inside the framework is not

difficult to track. It has been observed that the adsorbed
molecules tend to concentrate to the regions around the metal
clusters first and then the regions around the linkers.31,32_{ When }

the pressure is high enough, other concentrated regions of
adsorbates will appear around the two concentrated regions
mentioned above.33_{ We track the locations of adsorbates }

during the simulation using RASPA 2.0 and present the density distribution (represented by the dark green cloud) in Fig. 2 when 300 methane molecules are assigned in the unit structure of IRMOF-10 at 320 K.

To build a simple model that can simplify the calculations,
we further simplify the cuboids into square prisms (Fig. 1(c)) and
roughly divide the void space into three regions, i.e., the cubic
region around the corner with an evenly distributed attractive
potential of -*εz* (Fig. 1(d)), the region around the linker with an

evenly distributed attractive potential of -*εb* (Fig. 1(e)), and the

middle region, which is not affected by the attractive force of
the frameworks. Actually, the paddlewheel-fashion oriented
linkers create cavities with two different sizes34_{ where the }

densities of the adsorbates in those cavities are not the same. Since our model will calculate the average density in each attractive region that spans over other cells and cells of different sizes that exist periodically, it is not a necessity to discern the densities of different unit cells, and thus the simplified square prism linkers will be proven adequate.

**Table 1** The dimension of the simplified structures§

*L* *Lz* *Wz_L* *Wz_S* *Wz* *Lb* *Wb_L* *Wb_S* *Wb*
IRMOF-1 12.92 2.84
IRMOF-10 17.14 7.06
IRMOF-16 21.49 11.41
5.2 3.5
IRMOF-6 12.92 2.84 6.2 3.9
IRMOF-8 15.05 4.97 6.5 4.1
IRMOF-12 17.14 7.06 7.5 4.6
IRMOF-14 17.19
10.08 4.2 1.5 2.8
7.11 7.4
1.7
4.6
§_{Units: Å}

**Fig. 2** Density distribution in the IRMOF-10 when 300 CH4 molecules are assigned in the plotted structure space at 320 K

The dimension of the simplified structure is determined by
the real framework dimensions. According to Fig. 2, along the
direction of the linkers, the concentration difference of the
adsorbate on the upper and lower sides of the C2 atoms is
noticeable. In fact, the same phenomenon also occurs in other
IRMOFs. Therefore, we set the distance between the two C2
atoms on the linkers as the length of the linker prisms *Lb*. The

side of the corner cube *Lz* is the difference between the side of

the unit cell *L* and the linker length *Lb*. To calculate the widths

of the square prisms, we firstly calculate the long widths and
the short widths of the cuboids in Fig. 1(b), which shows the
geometrical similarities to the real frameworks. Since the rings
only have one layer of atoms, we set the average diameters of
the atoms on the rings as the short widths (*Wb_S*, *Wz_S*) of the

cuboids. For the long widths of the cuboids, we set the sum of
the H atom diameter and the average distance of the H atoms
pairs (Fig. 2) as the long widths (*Wb_L*, *Wz_L*). Because H atoms

are small and they appear at the boundary of the benzene rings,
they are not included in the calculation of the cuboids’ short
widths but are used for the calculation of the long widths. We
then set the average values of the long widths (*Wb_L*, *Wz_L*) and

the short widths (*Wb_S*, *Wz_S*) as the widths of the

corresponding square prisms (*Wb*, *Wz*) in Fig. 1(c). Table 1 lists

the parameters of IRMOFs mentioned in this paper, from which we can further conclude that the dimensions of the simplified structures are able to reflect the real materials, i.e., IRMOFs have the same corner clusters and the only difference of the linkers in IRMOF-1, IRMOF-10, and IRMOF-16 is the length.

**2.2 Simulations for verifying the simplifications**

Compared to the real conformations and properties of IRMOFs,
the simplified structures and attractive regions provide us with
a simple but clear understanding of the materials at the expense
of ignoring the details and later enable us to develop the
engineering model. However, it remains to be proven that the
simplified structures could work well in generating isotherms
that are in agreement with those obtained from experiments or
from simulations using more realistic interaction potentials at
atomistic level. To examine the applicability of the
simplifications, we conduct GCMC simulations for the
adsorption of methane in different IRMOFs using the simplified
structures. Square-well potential is applied to represent the
interactions among adsorbates and the interactions between
adsorbates and IRMOFs. The parameters of adsorbates are from
one version of the Statistical Associating Fluid Theory EOS (i.e.,
SAFT235_{), the parameters of which are obtained by fitting the }

saturated pressure and saturated liquid density data.36_{ These }

parameters can be found in Table 2, where *ε* represents the
attractive potential among molecules, *σ* is the molecule
diameter, *λσ* is the range of the potential well, and *k* is the

**Table 2** Parameters of adsorbates from SAFT2 equation of state

Boltzmann constant. The interaction between the adsorbate molecule and the surface of adsorbent has the following expression: ( 1 ) 𝑢𝑚𝑠=

## {

+∞ 𝑟𝑚𝑤< 1 2𝜎― 𝜀𝑧 𝑜𝑟 ― 𝜀𝑏 molecule center inside _{𝑎𝑡𝑡𝑟𝑎𝑐𝑡𝑖𝑣𝑒}_{𝑟𝑒𝑔𝑖𝑜𝑛}
0 _{attractive region & }molecule center outside_{𝑟}
𝑚𝑤>

1 2𝜎

where *rmw* is the distance of the adsorbate molecule center to

the surface of the simplified structure.

We assign at least 2 × 2 × 2 cells for the simulation box so that there are enough molecules to generate reliable results. Other simulation details can be found in our previous work.37

Considering that there is only van der Waals interaction
between a methane molecule and the structure atom, to keep
the properties of the simplified structures consistent with the
real materials, we assign the same attractive parameters to the
clusters of the same conformations in different IRMOFs, i.e., we
assign the same value of *εz* to the corner attractive regions of

different IRMOFs and the same value of *εb* and *δ* for linkers’

attractive regions of IRMOF-1, IRMOF-10, and IRMOF-16. Since
the attractive parameters *εz*, *εb*, and *δ* are not available, we

obtain them by fitting to realistic isotherms. The realistic isotherms are generated using RASPA 2.0 software. In this work, we choose the generic force field for the framework parameters, Transferable Potentials for Phase Equilibria (TraPPE) force field for adsorbate parameters, and Lennard-Jones (LJ) potential that is shifted to zero at the cutoff distance of 12Å with tail correction for the atomistic interactions.

Based on the description above, firstly, we fit the attractive
parameters *εz*, *εb*, and *δ*for IRMOF-1, IRMOF-10, and IRMOF-16.

Since they have the same conformations in linkers, i.e., benzene
rings, and the only difference among these three frameworks
are the linker length, their attractive parameters *εz*, *εb*, and *δ*

are the same in our model. This step is consistent with the
assumption that the clusters of the same conformations have
the same attractive parameters. For the other IRMOFs, we only
need to fit the two attractive parameters (*εb*, *δ*) for the linkers

with the *εz *known from the first step. Table 3 lists the fitted

parameters based on the isotherms generated by RASPA 2.0 at
250 K, which are then used for the adsorption predictions at
various temperatures in this section. The precisions of the
attractive potentials *εz* and *εb* are up to digit in the tens place

and the width of the attractive region around the linkers *δ* is up
to digit in the tenths place.

**Table 3** Simplified Simulation Parameters for CH4 adsorption in different IRMOFs

Corner Linker
*εz*/*k *(K) *εb*/*k *(K) *δ*
IRMOF-1
IRMOF-10
IRMOF-16
690 0.3
IRMOF-6 590 0.4
IRMOF-8 620 0.4
IRMOF-12 560 0.6
IRMOF-14
940
550 0.6
*ε*/*k *(K) *λ* *σ*(Å)
N2 96.4703 1.5144 3.1942
CO2 319.2744 1.3296 3.1788
CH4 130.5206 1.5942 3.2968

**Physical Chemistry Chemical Physics**

** ARTICLE**

Fig. 3(a) presents the predicted isotherms for methane
adsorption in different IRMOFs at 298 K. Fig. 3(b) presents the
predicted isotherms for methane adsorptions in IRMOF-8 and
IRMOF-12 at various temperatures. The good agreement of the
predicted isotherms with those obtained using RASPA 2.0
software proves that the simplified structures and the defined
attractive regions are able to reflect the adsorption
phenomenon in the real case. Furthermore, compared with the
real frameworks, the simplified structure uses simple prisms
with flat surfaces to represents groups of the atoms. The
complicated distribution of the adsorption sites analyzed by
Dubbeldam et al.33_{ is also replaced by simple attractive regions. }

Since these simplifications ignore the detailed locations of each atom on the framework and the detailed distribution of each adsorption site, the good performance of the model also suggests that adsorption isotherms are not sensitive to the detailed distribution of the attractive sites in the IRMOF structures and it is safe to ignore the geometrical details of the frameworks.

**2.3 Theoretical model**

The success of the application of square-well potential and the
simplified structures makes it possible to build an engineering
model for the prediction of the adsorption isotherms in IRMOFs.
Since the system is regarded to be in equilibrium, the chemical
potential of the adsorbed phase is equal to that of the bulk
phase. To predict the adsorbed amount in the simplified
structures, we equalize the chemical potentials of the adsorbate
in each attractive region to that of the bulk phase. We have
proven that in slit pores, the adsorbed amount in different
attractive regions can be predicted independently regardless of
the interactions among different regions.37_{ For the density in }

the middle region, which is not influenced by the attractive force of the framework, we approximate it using the density in the bulk. The chemical potential and density of the bulk phase are calculated using SAFT2.

The expression of the chemical potential of the fluid in the
attractive region is derived from the generalized van der Waals
canonical partition function *Q(T, V, N)*, as given below:37

( 2 ) 𝑄(𝑇,𝑉,𝑁) =

### (

𝑞 𝑁 𝑖𝑛𝑡 Λ3𝑁_{𝑁}

_{!}

### )

𝑉 𝑁 𝑓 exp### (

∫𝑇_{∞}𝐸𝑐𝑜𝑛𝑓 𝑘𝑇2𝑑𝑇

### )

( 3 ) 𝜇=―𝑘𝑇### [

∂ln (_{∂𝑁}𝑄)

### ]

𝑇,𝑉where *T* is the temperature, *V* is the volume,* N* is the number of
molecules, *qint* is the internal energy partition function for one

molecule, Λ is the de Broglie wavelength of the molecules, *Vf* is

the free volume of the hard-core fluid, *Econf* is the

configurational energy, and *µ* is the chemical potential.
According to the generalized van der Waals canonical partition
function and the expression for the chemical potential, two key
quantities for the calculation of the chemical potential in the
different attractive regions are free volume and configurational
energy.

The free volume in a certain attractive region is expressed as follows:

( 4 )

𝑉𝑓=𝑉 ― 𝑁 𝜌𝑚𝑎𝑥

where **max is the close-packed density of adsorbates in the

attractive region. Since the packing effects are expected to be
insignificant in real IRMOFs because the interaction with the
pore structure is not strongly felt throughout the space of the
frameworks,38_{ the close-packed density is approximated by that }

of the bulk, i.e., 2.

Since each cell in the IRMOF structure is tiny, it is unavoidable that different attractive regions overlap, which could lead to more complicated calculations. Because of the features of the simplified structure and attractive regions, only the linkers’ attractive regions could overlap. The configurational energy in a certain non-overlapping or overlapping attractive region is given by:

( 5 )

𝐸𝑐𝑜𝑛𝑓=― 𝑁

2𝑁𝑐𝜀 ― 𝑛𝑁𝜀𝑠

where the first term is to account for the energy generated by
the interaction among adsorbates and the second term is to
account for the energy from adsorbate-structure interaction in
the region. In Equation (5), *Nc* is the coordination number, *εs* is
(a) CH4 adsorption isotherms in different IRMOFs at 298 K.

(b) CH4 adsorption isotherms in IRMOF-8 and IRMOF-12 at different

temperatures.

**Fig. 3** Comparison of the isotherms generated by RASPA 2.0 (points) and the
simulation using simplified structures (lines)

the attractive potential of the adsorbate-structure interaction
(*εb* or *εz*), and *n* is the number of attractive potentials of the

adsorbate-structure interaction affecting the region. For a
non-overlapping region, the value of *n* is 1. In this work, we control
the sizes of the linkers’ attractive regions (*δ*) and limit them such
that triple or quadruple overlaps will not happen, and thus the
maximum value of *n* is 2. By doing this, we can avoid the
complex analysis regarding the shape of the regions with triple
or quadruple overlaps and the calculation becomes simpler. The
distribution of the attractive regions and the occurrence of
overlaps are depicted and explained in the supplementary
material. As shown later, although triple overlaps are avoided,
the isotherms obtained from both the simplified simulation and
the modeling are still in agreement with those obtained from
RASPA 2.0.

By assuming uniform density in each region, the coordination number of a region can be obtained from:

( 6 )

𝑁𝑐= 4𝜋𝜌∫𝑔(𝑟,𝜌,𝑇)𝑟2𝑑𝑟

where *g* is the radial distribution function and ** is the number
density in the region. As in our previous work,37_{ the radial }

distribution function used in the derivation of the coordination
number is approximated by the low-density radial distribution
function for square-well fluid, i.e., *g*(*r*, ** = 0, *T* ):

( 7 )

𝑔(𝑟) =

### {

0 𝑟<𝜎 𝑒𝑥𝑝

### (

_{𝑘𝑇}𝜀

### )

𝜎 ≤ 𝑟 ≤ 𝜆𝜎1 𝑟>𝜆𝜎

where *r* is the center to center distance between the central
molecule and the molecule around it.

The expression of the coordination number was shown to simplify to:37

( 8 )

𝑁𝑐=𝐶𝑒𝑥𝑝

### (

𝜀 𝑘𝑇### )

𝜌∗where *C* represents the reduced volume of the potential well of
a molecule within the attractive region and ***_{ is the reduced }

density (=**3_{). Unlike the prediction of the coordination }

number for molecules in slit pores, the reduced volume *C* is no
longer a constant at different locations in each attractive region
of the simplified IRMOF structure. However, since the volume
of each attractive region is small, we set *C* to be a constant and
will check in this section if high accuracy of isotherm prediction
can still be achieved. Since the range of *δ* is controlled such that
triple overlaps will not happen, the volume of the overlapped
regions could be even smaller than that of a methane molecule
in some frameworks. Thus, we can safely set the reduced
volume constant in these regions to zero, which means we
neglect the existence of adsorbate-adsorbate interaction in the
overlapping regions.

From the above analysis, the expression of the chemical potential of an attractive region is:

𝜇=𝑅𝑇

### [

𝑙𝑛### (

Λ ( 9 ) 3_{𝑁}𝑎𝑣 𝑣 ― 𝑏

### )

+ 𝑏 𝑣 ― 𝑏### ]

― 2𝑎 𝑣 ― 𝑁𝑎𝑣𝑛𝜀𝑠where* Nav* is the Avogadro number, *R* is the gas constant (=
*kNav*), *v* is the molar volume in the region, and *a* and *b* are the

van der Waals parameters in our model given by:

( 10 ) 𝑎=𝑁2 𝑎𝑣 𝐶𝜎 2𝑘𝑇

### [

𝑒𝑥𝑝### (

𝜀 𝑘𝑇### )

―1### ]

( 11 ) 𝑏=_{𝜌}𝑁𝑎𝑣 𝑚𝑎𝑥

In Equation (10), *C* = *Cz* for the attractive region at the

corner, *C* = *Cb*for the non-overlapping attractive region around

linker, and *C* = 0 for the overlapping linkers’ attractive region.
To check the applicability of constant reduced volumes, in
this section we directly fit the reduced volume constants in
non-overlapping attractive regions using the densities in those
regions obtained from simplified simulation at one temperature
and apply them to predict the adsorbed amounts at other
temperatures. Fig. 4 presents the predicted adsorbed amounts
of CH4 in different regions of IRMOF-10 and the overall

performance of the model in predicting isotherms at 298 K by using the reduced volumes fitted from the densities of the attractive regions at 250 K and the other parameters from Table 3. It is noticeable that the underestimation of the overall adsorbed amount at high pressure is mainly because of the underestimation of the density in the middle region, where the density is assumed to be the same as that in the bulk phase. In real case, when the pressure is high, the density in the middle region starts to deviate from that of the bulk phase. Nevertheless, we still can conclude that the model works well in predicting the densities in attractive regions, and the reduced volume constants fitted from the isotherm at one temperature can be applied to the prediction of isotherms at other temperatures. The error at high pressures will be fixed and explained in the next section.

**3. Results and Applications**

The previous sections indicate that the model can predict the
densities of different attractive regions by fitting the reduced
volumes. However, it would be a time-consuming process if we
obtain the five parameters (*εz*, *εb*, *δ*, *Cz*, *Cb*) by conducting

points are obtained from simplified simulation; lines are model prediction
**Fig. 4** Adsorbed amounts of methane in different regions for IRMOF-10 at 298 K

**Physical Chemistry Chemical Physics**

** ARTICLE**

simplified simulations. In fact, we can obtain all the parameters by directly fitting the model to real isotherms.

Figs. 5(a) and 5(b) are the predicted isotherms of CH4 based

on the parameters fitted to the isotherms at 250 K, Figs. 5(c) and 5(d) are the predicted isotherms of N2 based on the

parameters fitted to the isotherms at 200 K, and Figs. 5(e) and 5(f) are the predicted isotherms of CO2 based on the parameters

fitted to the isotherms at 298 K. These parameters are listed in

Table 4. The predicted adsorbed amounts of different adsorbates in different IRMOFs are in good agreements with the

data generated by RASPA 2.0, and the different types of
isotherms (IUPAC adsorption Type I and Type V) 39_{ are well }

captured.

For quadrupolar gases, such as N2 and CO2, the interactions

between the adsorbate and IRMOFs are not only van der Waals interaction, but also Coulombic interactions, which play an

(a) CH4 in different IRMOFs at 280 K (b) CH4 in IRMOF-1 at various temperatures

(f) CO2 in IRMOF-1 at various temperature

(e) CO2 in different IRMOFs at 320 K

(d) N2 in IRMOF-1 at various temperatures

(c) N2 in different IRMOFs at 220 K

important role because of the partial charges of the IRMOF atoms. The influence of Coulombic interactions, in a macroscopic point of view, is evident from the high densities of adsorbates around the corner and linker. Therefore, this will not influence the implementation of the model since the distribution of the quadrupolar molecules inside the structures is similar to that of non-polar adsorbates,33 which means that predicting the isotherms can still be achieved by predicting the adsorbed amount in each attractive region. In other words, the influence of the Coulombic interaction does not need additional treatment and the model, which only considers square-well potentials, works as well as it does for non-polar molecules. No additional parameters or model modifications are needed.

From Fig. 5, we find that the predicted isotherms are in
agreement with the results obtained from RASPA 2.0. This fact
further confirms that the fitted attractive parameters absorb
the influence of the interactions among different attractive
regions. For comparison, predictions of methane adsorption in
IRMOF-6 and IRMOF-8 at 298 K have been attempted using SL
and PHSC EOS,26_{ but the results were found to be }

unsatisfactory.

As mentioned at the beginning of this paper, for the same kind of materials, the isotherm at the same temperature can vary if the materials are synthesized by different research groups. Although the interaction potential used in doing molecular simulation is close to the real value, errors still exist when compared with the experimental data, because materials synthesized in the lab are not as ideal as that in the simulation and the purity of the materials are different to a certain degree due to different experimental conditions. Therefore, if we want to predict the isotherms of a material synthesized in a particular lab, doing molecular simulation or using adsorption models with parameters obtained from data of other labs/experiments will

not be able to accurately predict its isotherms. The model
proposed in this work just needs an isotherm at one
temperature to find the parameters, and the isotherms at other
temperatures can be predicted accurately. Fig. 6 presents the
performance of our model in predicting isotherms. The
scattered points are the experimental data.40_{ For the }

adsorption of CH4 in IRMOF-1, which have lower values than

those obtained from RASPA 2.0, and are very different from
those obtained in other experimental works.41,42_{ We fitted the }

five parameters in our model to the isotherm at 248.5 K (*εz*/*k *=

921.1 K , *εb*/*k* = 574.1 K,*δ* = 0.35, *Cz* = 4.0, *Cb* = 5.1) and use this

set of parameters to predict the isotherms at other temperatures. The excellent agreement with the experimental data demonstrates that our model can be a powerful tool for predicting the isotherms of real materials.

**Table 4** Fitted Parameters for CH4, CO2, and N2 adsorption in different IRMOFs

*εz*/*k *(K) *εb*/*k *(K) *δ* *Cz* *Cb*
IRMOF-1 956.2 642.5 0.35 4.14 5.40
IRMOF-6 828.0 1017.0 0.29 4.88 4.68
IRMOF-8 857.0 637.2 0.49 5.03 5.08
IRMOF-10 799.7 573.5 0.60 3.87 4.32
IRMOF-12 860.1 654.5 0.61 5.00 4.37
IRMOF-14 736.5 666.0 0.62 5.50 4.21
CH4
IRMOF-16 707.1 472.5 0.79 4.13 3.83
IRMOF-1 1070.0 835.0 0.36 1.79 2.16
IRMOF-6 1163.0 986.3 0.37 1.71 1.79
IRMOF-8 834.2 784.5 0.56 2.49 2.10
IRMOF-10 846.8 684.7 0.63 2.20 1.99
IRMOF-12 835.9 759.7 0.66 2.49 2.12
IRMOF-14 828.2 756.8 0.68 2.52 2.15
CO2
IRMOF-16 918.8 610.0 0.62 1.67 2.20
IRMOF-1 741.2 559.5 0.31 2.11 3.80
IRMOF-6 838.4 608.9 0.31 2.10 3.30
IRMOF-8 707.0 510.8 0.44 3.28 3.49
IRMOF-10 685.1 475.4 0.45 2.03 3.17
IRMOF-12 728.2 517.3 0.49 4.21 3.32
IRMOF-14 714.9 509.3 0.50 4.32 3.37
N2
IRMOF-16 668.5 436.7 0.51 1.62 2.76

**Fig. 6** Experimental isotherms (points) and predicted isotherms (lines) for CH4

**Physical Chemistry Chemical Physics**

** ARTICLE**

**4. Conclusions**

A simple engineering model for adsorption derived from the Generalized van der Waals partition function is proposed to describe the isotherms of light gas adsorption in IRMOFs. The model is developed by making reasonable simplification to the structures of IRMOFs and defining important attractive regions of square-well potential. The simplification of the structures is based on the geometries of the accessible surfaces and the dimensions of the frameworks. The locations of the attractive regions are defined by examining the distribution of the concentrated adsorbates.

The reliability of the simplification is first verified by conducting molecular simulations. Grand Canonical Monte Carlo (GCMC) simulations using both the simplified structures with square-well potentials and the complete atomic structures with Lennard-Jones and Coulombic potentials are performed and compared. Simulations based on Lennard-Jones potential are conducted as a reference to the simplified simulation and the adsorption model. We demonstrate that the simplified simulation can generate the adsorption isotherms of different IRMOFs with high accuracy and the model can predict the adsorbed amounts in different attractive regions accurately. Given one of the isotherms, we can fit the five parameters of the model and use them to accurately predict the isotherms at other temperatures. For the adsorption of quadrupolar molecules, the effect of the columbic interactions can be adsorbed by the square-well potential and the adsorption isotherms in IRMOFs can still be predicted accurately.

It is also demonstrated that the application of the model is not limited to the adsorption prediction in ideal IRMOF structures, i.e., the structures used in simulations, but also in frameworks synthesized by experiments, which are imperfect in purity and structure completeness. The predicted isotherms using our model can accurately match those obtained from experiments.

**Conflicts of interest**

There are no conflicts to declare.

**Acknowledgements**

This work is supported by the State of Wyoming and the Department of Energy (DE-PI0000017).

**References**

1 A. U. Czaja, N. Trukhan and U. Muller, *Chemical Society *
*Reviews*, 2009, **38**, 1284-1293.

2 J. R. Li, R. J. Kuppler and H. C. Zhou, *Chemical Society Reviews*,
2009, **38**, 1477-1504.

3 T. Duren, Y. S. Bae and R. Q. Snurr, *Chemical Society Reviews*,
2009, **38**, 1237-1247.

4 R. B. Getman, Y. S. Bae, C. E. Wilmer and R. Q. Snurr, *Chemical *
*Reviews*, 2012, **112**, 703-723.

5 A. K. Rappe, C. J. Casewit, K. S. Colwell, W. A. Goddard and W.
M. Skiff, *Journal of the American Chemical Society*, 1992, **114**,
10024-10035.

6 S. L. Mayo, B. D. Olafson and W. A. Goddard, *Journal of *
*Physical Chemistry*, 1990, **94**, 8897-8909.

7 S. Amirjalayer and R. Schmid, *Journal of Physical Chemistry C*,
2008, **112**, 14980-14987.

8 L. C. Lin, K. Lee, L. Gagliardi, J. B. Neaton and B. Smit, *Journal *
*of Chemical Theory and Computation*, 2014, **10**, 1477-1488.
9 O. Engkvist, P. O. Astrand and G. Karlstrom, *Chemical Reviews*,

2000, **100**, 4087-4108.

10 T. Mueller and G. Ceder, *Journal of Physical Chemistry B*, 2005,

**109**, 17974-17983.

11 A. L. Dzubak, L. C. Lin, J. Kim, J. A. Swisher, R. Poloni, S. N.
Maximoff, B. Smit and L. Gagliardi, *Nature Chemistry*, 2012, **4**,
810-816.

12 P. L. Liao, R. B. Getman and R. Q. Snurr, *Acs Applied Materials *
*& Interfaces*, 2017, **9**, 33484-33492.

13 L. J. Chen, C. A. Morrison and T. Duren, *Journal of Physical *
*Chemistry C*, 2012, **116**, 18899-18909.

14 C. E. Wilmer, M. Leaf, C. Y. Lee, O. K. Farha, B. G. Hauser, J. T.
Hupp and R. Q. Snurr, *Nature Chemistry*, 2012, **4**, 83-89.
15 C. Altintas and S. Keskin, *Chemical Engineering Science*, 2016,

**139**, 49-60.

16 E. Haldoupis, S. Nair and D. S. Sholl, *Journal of the American *
*Chemical Society*, 2012, **134**, 4313-4323.

17 R. Krishna, *Rsc Advances*, 2017, **7**, 35724-35737.

18 Z. W. Qiao, Q. S. Xu, A. K. Cheetham and J. W. Jiang, *Journal of *
*Physical Chemistry C*, 2017, **121**, 22208-22215.

19 H. Frost, T. Duren and R. Q. Snurr, *Journal of Physical *
*Chemistry B*, 2006, **110**, 9565-9570.

20 J. L. Mendoza-Cortes, S. S. Han, H. Furukawa, O. M. Yaghi and
W. A. Goddard, *Journal of Physical Chemistry A*, 2010, **114**,
10824-10833.

21 H. D. Zhang, P. Deria, O. K. Farha, J. T. Hupp and R. Q. Snurr,

*Energy & Environmental Science*, 2015, **8**, 1501-1510.
22 K. Sillar, A. Hofmann and J. Sauer, *Journal of the American *

*Chemical Society*, 2009, **131**, 4143-4150.

23 K. Sillar and J. Sauer, *Journal of the American Chemical Society*,
2012, **134**, 18354-18365.

24 S. J. Alesaadi and F. Sabzi, *International Journal of Hydrogen *
*Energy*, 2014, **39**, 21076-21082.

25 S. J. Alesaadi and F. Sabzi, *International Journal of Hydrogen *
*Energy*, 2014, **39**, 14851-14857.

26 M. Tahmooresi and F. Sabzi, *Journal of Inorganic and *
*Organometallic Polymers and Materials*, 2015, **25**, 1298-1304.
27 V. M. Trejos, A. Martinez and A. Gil-Villegas, *Fluid Phase *

*Equilibria*, 2018, **462**, 153-171.

28 M. Eddaoudi, J. Kim, N. Rosi, D. Vodak, J. Wachter, M. O’Keeffe
and O. M. Yaghi, *Science*, 2002, **295**, 469–472.

29 D. Dubbeldam, S. Calero, D. E. Ellis and R. Q. Snurr, *Molecular *
*Simulation*, 2016, **42**, 81-101.

30 D. Fairen-Jimenez, N. A. Seaton and T. Duren, *Langmuir*, 2010,

**26**, 14694-14699.

31 Q. T. Ma, Q. Y. Yang, C. L. Zhong, J. G. Mi and D. H. Liu,

*Langmuir*, 2010, **26**, 5160-5166.

32 N. S. Suraweera, R. C. Xiong, J. P. Luna, D. M. Nicholson and D.
J. Keffer, *Molecular Simulation*, 2011, **37**, 621-639.

33 D. Dubbeldam, H. Frost, K. S. Walton and R. Q. Snurr, *Fluid *
*Phase Equilibria*, 2007, **261**, 152-161.

34 T. Duren, L. Sarkisov, O. M. Yaghi and R. Q. Snurr, *Langmuir*,
2004, **20**, 2683-2689.

35 S. P. Tan, X. Y. Ji, H. Adidharma and M. Radosz, *Journal of *
*Physical Chemistry B*, 2006, **110**, 16694-16699.

http://www.webbook.nist.gov/chemistry/, (accessed July 2018).

37 L. L. Kong and H. Adidharma, *Chemical Engineering Science*,
2018, **177**, 323-332.

38 T. Duren and R. Q. Snurr, *Journal of Physical Chemistry B*,
2004, **108**, 15703-15708.

39 K. S. W. Sing, D. H. Everett, R. A. W. Haul, L. Moscou, R. A.
Pierotti, J. Rouquerol and T. Siemieniewska, *Pure and Applied *
*Chemistry*, 1985, **57**, 603-619.

40 J. A. Mason, M. Veenstra and J. R. Long, *Chemical Science*,
2014, **5**, 32-51.

41 D. Saha, Z. B. Bao, F. Jia and S. G. Deng, *Environmental Science *
*& Technology*, 2010, **44**, 1820-1826.

42 W. Zhou, H. Wu, M. R. Hartman and T. Yildirim, *Journal of *
*Physical Chemistry C*, 2007, **111**, 16131-16137.